OPEN SUBJECT AREAS: GRAPHENE ELECTRONIC PROPERTIES AND DEVICES NANOSCALE MATERIALS
Received 3 September 2014 Accepted 3 November 2014 Published 26 November 2014
Correspondence and requests for materials should be addressed to P.L. ([email protected]
Flexible transparent graphene/polymer multilayers for efficient electromagnetic field absorption K. Batrakov1, P. Kuzhir1, S. Maksimenko1, A. Paddubskaya1, S. Voronovich1, Ph Lambin2, T. Kaplas3 & Yu Svirko3 1
Research Institute for Nuclear Problems, Belarusian State University, Minsk 220030, Belarus, 2Physics Department, Universite´ de Namur, 61 Rue de Bruxelles, B-5000 Namur, Belgium, 3Department of Physics and Mathematics, University of Eastern Finland, Joensuu FI-80101, Finland.
Thanks to its high electrical conductivity, a graphene plane presents a good shielding efficiency against GHz electromagnetic radiations. Several graphene planes separated by thin polymer spacers add their conductivities arithmetically, because each of them conserves the intrinsic properties of isolated graphene. Maximum absorption of radiations for frequency around 30 GHz is achieved with six separated graphene planes, which is the optimum number. This remarkable result is demonstrated experimentally from electromagnetic measurements performed in the Ka band on a series of multilayers obtained by piling 1, 2, 3 … graphene/PMMA units on a silica substrate. Theoretical calculations convincingly explain the observed absorption and transmission data in the GHz domain. It is concluded that graphene/PMMA multilayers can be used as an efficient optically transparent and flexible shielding media.
icrowave is the ultimate range for open space communication. The rapid growth of satellite data transmission in last decades, reinforced by the Internet traffic, makes inevitable the overcrowding of the spectral bands allocated to the different communication channels. Along with the increasing density of emitters in the environment, this has made the Electromagnetic Compatibility (EMC) an important issue1. EMC rules require that each new equipment have adequate immunity in order to function consistently and reliably, be resilient to major electromagnetic (EM) disturbances, and coexist with other equipments. In order to meet these requirements, there is a real need for new materials to be used as coating layers, shields and filters in future nanoelectronic devices. These materials must have high electrical conductivity to achieve a good EM shielding effectiveness, defined as the reciprocal of the transmission factor. It is worth noting, however, that EM radiations reflected from the protective coatings do contribute to the microwave pollution. Consequantly, absorption rather than reflection losses should dominate the EM attenuation in the new materials. In addition, protection of the future nanodevices require submicron thick shields, making useless conventional conductive coatings capable to produce an EM attenuation of up to 3 dB/mm. The challenging problem of the electromagnetic interference (EMI) protection at the nanoscale may be resolved if one exploits the unusual electronic properties of graphene. Very recently we have proposed microwave shielding based on nanometrically thin pyrolytic carbon (PyC) films2 composed of intertwined graphene ribbons. Specifically, 30–35 nm thick PyC films secure about 60% attenuation at 28 GHz mainly due to absorption of the EM radiations. The absorption efficiency of the EM protective coating can be increased even further by replacing PyC with few-layer graphite (FLG), which is capable to absorb 40% of microwave radiation at a thickness of only 5 nm3. Interlayer interactions affect the band structure of FLGs near the Fermi level in a qualitative way: compared to graphene, the dispersion of the p bands is no longer linear around the Dirac points4. This modification has direct consequences on properties such as the electrical conductivity that crucially depend on the topology of the Fermi surface5. When the distance between the graphene layers exceeds that realized in graphite by a fraction of a nanometer and more, the interlayer interaction plays no role anymore. In these conditions, the measured sheet conductivity increases in proportion to the number of graphene layers6. Therefore, one may expect that by separating graphene layers from one another in a controlled way by dielectric spacers, one can create a nano-metamaterial with enhanced shielding efficiency. This approach has been recently theoretically discussed in terms of an ultra-broadband THz absorber7, in which high-order surface plasmon resonances can be introduced by patterning graphene layers with micrometer periodicity. SCIENTIFIC REPORTS | 4 : 7191 | DOI: 10.1038/srep07191
Figure 1 | Schematic representation of graphene sandwich fabrication, consisting of a number of repeating steps, and final graphene/PMMA multilayer structure containing here four graphene sheets (the thickness of the different layers were not drawn in scale). The lateral dimensions of the samples are 7.2 mm 3 3.4 mm.
In this paper we demonstrate both experimentally and theoretically that a stack of PMMA thin films sandwiching graphene sheets between them has remarkable microwave EMI shielding effectiveness. Specifically, in the Ka band (frequency range between 26.5 and 40 GHz), strong absorption of the EM radiation can be achieved without pre-patterning of the graphene whose overall thickness of two nanometers is enough to absorb 50% of the incident EM power.
Results Experiment. Fig. 1 shows schematically the graphene/PMMA multilayers produced for EM shielding analysis. The thickness of the PMMA spacers is in the range 600–800 nm. These sandwich structures were produced as follows. The first graphene layer was synthesized by chemical vapor deposition (CVD) at 1000uC in methane atmosphere on a copper foil. It was next covered by a PMMA layer obtained by spin coating, after what Cu was wet etched in ferric chloride. The obtained PMMA film with its graphene layer was washed in distilled water, placed on a quartz (fused silica) substrate and dried. The very same procedure was repeated several times, each newly-produced graphene/PMMA unit being deposited on top of the stack obtained at the previous step. This procedure allowed us to fabricate sandwich multilayers containing several graphene sheets. The SEM image reproduced in Fig. 2(a) demonstrates that the PMMA-based transfer technique8 allowed us to produce a continuous graphene sheet with a tiny number of holes. In addition, the
optical transmittance of a graphene layer without the carrier PMMA film, taking out the response of the bare substrate (see Fig. 2(b)), was 97.8% at 800 nm, which is only 0.3% below that expected for a single graphene layer9. This measurement indicates that areas covered by bi- and multi-layer graphene are small. The Raman spectrum shown in Fig. 2(c) presents sharp G and 2D lines. More specifically, a sharp G peak (GFWHM , 20 cm21) and the absence of D peak point to a high crystallinity of the graphene layer10. Furthermore, the 2D line peaks at 2688 cm21 is typical for graphene monolayer10. However, the 2D peak is slightly broader (,40 cm21) than expected for a graphene monolayer (30 cm21), indicating some presence of bilayer graphene. Microwave measurements were made with a scalar network analyzer R2-408R (ELMIKA, Vilnius, Lithuania). The setup includes a sweep generator, a waveguide reflectometer and an indicator unit. The IEC 62431:2008(E) standard for reflectivity measurements of EM materials was used. The frequency stability of the oscillator was controlled at the 1026 level by a frequency meter. The power used was 7.0 mW 6 10 mW. The error on the measured EM attenuation was 7% in the range 0 to 240 dB. The ratios of transmitted/ input (S21) and reflected/input (S11) signals were measured at 30 GHz before and after insertion of the specimen into the waveguide. The lateral dimensions of the samples fitted precisely the waveguide 7.2 3 3.4 mm2 cross section. The transmission (T) and reflection (R) coefficients of graphene/ PMMA sandwich structure consisting of one to four graphene layers
Figure 2 | (a) SEM picture of a graphene layer transferred from copper foil to a silica substrate. (b) Wavelength dependence of the visible-UV transmittance of a graphene layer on silica substrate corrected from that of the bare substrate). (c) Raman spectrum of the graphene layer. SCIENTIFIC REPORTS | 4 : 7191 | DOI: 10.1038/srep07191
Figure 3 | Absorption (a,b) and transmission (c) coefficients at 30 GHz of graphene/PMMA multilayers on silica containing N~0 4 graphene/ PMMA units. In panel (a), the incident EM waves come from the side of the silica substrate (upward orientation of the graphene/PMMA sandwiches), in (b) they come from the other side of the samples (downward). The upward or downward orientation of the samples has no influence on the transmission. Both measured and calculated (eq. 5) values are represented.
were deduced from the measured S parameters. The measurements were performed for the two possible normal orientations of the samples: in the first orientation, the guided EM wave enters the sample through the silica substrate and leaves it from the graphene/PMMA side (upward), the second orientation (downward) being just the reverse. Fig. 3(a) displays the variation of the absorption coefficient A 5 1 2 T 2 R versus the number N of graphene/PMMA units for the upward geometry: the absorbance varies between 25% (one graphene layer) to 48% (four graphene layers). The silica substrate and PMMA being non-absorbing in the Ka band, all the incident EM power is absorbed by the graphene layers. The absorption coefficient is approximately a factor of 1.2 smaller for the downward geometry (Fig. 3(b)) compared to the upward geometry: A varies between 21% (one graphene layer) to 40% (four graphene layers). The transmission coefficient (Fig. 3(c)) is the same for both orientations of the sample. It decreases monotonously between 58% and 25%, the silica substrate itself reflects 21% of the incident radiation. Theory. Before proceeding to a quantitative analysis of these measurements, it is worth understanding why graphene is so good in absorbing EM radiations in the Ka band. Indeed, a single graphene layer was shown to absorb 21 to 25% of the incident radiation3, which is a lot for a one-atom thick material. For a qualitative explanation, it is sufficient to refer to the Fresnel formulas for the transmission and reflection of a plane wave at the interface between two dielectric media when the interface sustains an infinitely thin –at the scale of the incident wavelength– conducting layer. In normal incidence, the electric and magnetic fields are parallel to the interface. Their amplitudes must satisfy the boundary conditions Ei zEr ~Et and Hi zHr ~Ht zsEt
where the subscripts i, r, and t refer to the incident, reflected, and transmitted waves, respectively. The last term in the second relation is the surface current density induced by the electric field in the interfacial layer with sheet conductance s. Starting from the boundary conditions (eq. 1), the reflectance R, transmittance T and absorbance A of the interfacial layer between media with refractive indices n1 and n2 are readily derived11,12. In particular, Re s 4n1 4n1 n2 0 n2 c T~ ð2Þ 2 and A~ 2 s n1 zn2 z 0 c n1 zn2 z s0 c SCIENTIFIC REPORTS | 4 : 7191 | DOI: 10.1038/srep07191
where 0 is the vacuum permittivity and c the speed of light in vacuum. Both T and A are functions of the real and imaginary parts of the interfacial layer conductance. The maximum of absorbance is reached when Im s 5 0 and Re s~ðn1 zn2 Þ 0 c. The maximum value of A is n1/(n1 1 n2). When EM radiations propagating in air (n1 5 1) enter a dielectric medium coated by a thin conductive layer (analogue of the downward sample orientation, Fig. 3(b)), the bigger the refractive index n2 of the dielectric, the lower the absorbance. However if EM radiations propagate in the opposite direction, i.e. from the dielectric medium to air (n2 5 1) (analogue of the upward sample orientation, Fig. 3(a)), the bigger the refractive index n1 of the dielectric, the higher the absorbance. In particular the absorbance can exceed 50% when n1 . n211. Reaching maximum absorption requires Re s= 0 c